Corrosive microenvironments at lead solder surfaces arising from galvanic corrosion
Environ. Sci. Technol. 2010, 44, 7076–7081
which is consistent with observations of Reiber et al. in
Corrosive Microenvironments at continuous ﬂow testing of waters to which sulfate was added
Lead Solder Surfaces Arising from (11, 12). Later practical data demonstrated very strong links
between the reported 90th percentile lead at certain utilities
Galvanic Corrosion with Copper Pipe and the CSMR (13), as well as elevated CSMR due to changing
coagulant chemical from aluminum sulfate to either ferric
chloride or polyaluminum chloride (2). Increased leaching
CAROLINE K. NGUYEN,
and galvanic corrosion of lead solder at higher CSMR has
KENDALL R. STONE, ABHIJEET DUDI,
also been unambiguously demonstrated at bench scale by
AND MARC A. EDWARDS*
Dudi et al. (14) and Edwards et al. (2). Practical case studies
Civil and Environmental Engineering Department, Virginia by Nguyen et al. found a correlation between the CSMR and
Tech, 407 Durham Hall, Blacksburg, Virginia 24061
lead release from galvanic solder in a range of waters (15).
Although the practical link between higher CSMR and
Received May 4, 2010. Revised manuscript received August higher lead leaching from solder is now well established in
9, 2010. Accepted August 11, 2010. the literature, the precise mechanism(s) for the sustained
attack due to chloride have never been elucidated. The goal
of this work was to unambiguously identify the key steps by
which galvanic corrosion currents can cause persistent
As stagnant water contacts copper pipe and lead solder dissolution of lead bearing materials connected to copper
(simulated soldered joints), a corrosion cell is formed between pipe. Conceptually, when lead is physically connected to
the metals in solder (Pb, Sn) and the copper. If the resulting copper, the lead surface is anodic and the rate of lead
galvanic current exceeds about 2 µA/cm2, a highly corrosive corrosion is accelerated. The free lead (Pb2+) released to the
microenvironment can form at the solder surface, with pH < 2.5 water is a Lewis acid, which decreases pH upon removal of
and chloride concentrations at least 11 times higher than OH- ions from the water via formation of soluble complexes
bulk water levels. Waters with relatively high chloride tend to or insoluble precipitates that contain OH- (14). Speciﬁcally,
sustain high galvanic currents, preventing passivation of the release of 50 mg/L Pb(II) can reduce the pH from 8 to 5.8 in
solder surface, and contributing to lead contamination of potable water with 20 mg/L alkalinity as CaCO3. However, if the same
mass of tin, which is a stronger Lewis acid than lead, were
water supplies. The total mass of lead corroded was consistent
released from 50:50 (by weight) Pb/Sn solder, the pH is
with predictions based on the galvanic current, and lead predicted to decrease to 2.9-3.5. A higher alkalinity might
leaching to water was correlated with galvanic current. If the tend to buffer the pH drop (14). Because the resulting low
concentration of sulfate in the water increased relative to pH can hinder formation of passive ﬁlms on the lead solder
chloride, galvanic currents and associated lead contamination surfaces, it could contribute to self-perpetuation of the attack
could be greatly reduced, and solder surfaces were readily and associated water contamination.
passivated. Another factor affecting corrosion is the migration of
anions such as chloride or sulfate to the lead anode surface,
which is necessary to balance electroneutrality of the released
Introduction Pb2+ or Sn2+. The increased concentration of anions at anode
Seemingly innocuous changes in chemistry can sometimes surfaces versus the concentration in bulk water is well
dramatically increase the likelihood of lead contamination understood, and has even been considered as a means of
from lead pipes, soldered joints, and lead-bearing brass (1-5). removing anionic contaminants from soils via electromi-
In some cases, the changes have resulted in exceedances of gration (16, 17). The net concentration of anions at anode
lead levels speciﬁed in the United States Environmental surfaces can be predicted using a one-dimensional model
Protection Agency (U.S. EPA) Lead and Copper Rule (LCR), that accounts for anion migration and diffusion (18). Key
elevated blood lead, and even lead poisoning (2, 6-8). One results of this model illustrate two extremes in behavior that
important subset of inﬂuential treatment changes, as high- are relevant to the current application. Speciﬁcally, if the
lighted by Edwards et al., involves dramatically increased current density exceeds about 2 µA/cm2, net anion transport
lead release from lead solder:copper joints that are triggered is toward the anode (anion migration toward the anode is
by increases in the chloride-to-sulfate mass ratio (CSMR ) much greater than diffusion of anions away from the anode),
mg/L chloride divided by mg/L sulfate) of the water supply resulting in accumulation of Cl- or SO42- at the anode surface
(2). Some of the resulting problems with elevated lead relative to bulk water (16). In other words, when this threshold
occurred while utilities practiced optimized corrosion control of current density is exceeded, the anion concentration factor
using orthophosphate inhibitors (2). (CF ) anion concentration near the anode surface divided
The nature and importance of galvanic corrosion on by the anion concentration in the bulk water) becomes very
contamination of water from lead plumbing was ﬁrst detailed high. At another extreme, if the current density is very low,
by Oliphant and Gregory (9, 10). These authors discovered net transport of anions toward the anode is low relative to
that waters with a CSMR above about 0.6 had very high and diffusion of anions away from the anode, reducing the net
persistent galvanic currents ﬂowing between copper pipe CF of anions near the anode surface. In the experimental
and lead solder. The lead solder anode, sacriﬁced by the data of Horng using a copper anode, sulfate was concentrated
connection to the cathodic copper, was suspected to cause at the anode surface by a factor of 1.4-5 when the current
severe lead contamination of potable water (9, 10). If the density increased from 10 to 25 µA/cm2 (16).
CSMR of the water was lower, galvanic currents between In general, the range of chloride and sulfate concentrations
lead solder and copper decreased markedly with time (9, 10), commonly encountered in potable water are not expected
to inﬂuence lead solubility via formation of either soluble
* Corresponding author phone: (540)231-7236; fax: (540)231-7916; complexes or lead precipitates (19). However, if these ions
e-mail: firstname.lastname@example.org. were to become concentrated at the surface of the anode,
7076 9 ENVIRONMENTAL SCIENCE & TECHNOLOGY / VOL. 44, NO. 18, 2010 10.1021/es1015185 2010 American Chemical Society
Published on Web 08/25/2010
connected to the copper pipes via copper wires. The
apparatus was oriented vertically so that the solder, lead,
and tin wires were at the bottom. Pure lead and tin wires
were also evaluated in this study to identify tendencies
speciﬁc to each metal present in 50:50 Pb/Sn solder.
Water Chemistry. The pipes were exposed to different
water chemistries to simulate real-world problems observed
in practice (Table 1). Raw water from the utility in Case Study
1 was received and treated at bench scale with the speciﬁed
coagulants and disinfectants to simulate full-scale treatment
(Table 1). In Case Study 2, treated water, but prior to
disinfection, was received at Virginia Tech from Utility 2.
Water for Case Study 3 was treated using reagent grade
chemicals. The chloride and sulfate concentrations were
selected to represent the range of chloride and sulfate
concentrations quantiﬁed in potable water. The pH, inhibitor
dose, and disinfectant concentrations were adjusted for all
FIGURE 1. Schematic of copper joint macrocell used in case waters prior to exposure to the macrocells. Details of the
bench scale treatment for each case study are provided in
the Supporting Information (SI).
signiﬁcant impacts on lead solubility at the anode surface Experimental Protocol. The water in the pipes was
are predicted. Speciﬁcally, at high concentrations, chloride changed three times per week using a “dump-and-ﬁll”
is predicted to form soluble complexes with lead and increase
protocol (2). Each water condition was tested in triplicate.
its solubility, whereas sulfate can form a relatively insoluble
Water left stagnant in the pipes for two to three days was
precipitate with lead and decrease its solubility (20, 21). Work
collected and analyzed for metals at the end of each week.
by Guo with polarized lead electrodes suggested that insoluble
Although the average stagnation time in buildings between
metal salts, such as PbSO4 or other salts containing multi-
valent anions, could passivate the scale from the active state ﬂow events is on the order of 30 min, a longer stagnation
even under highly acidic conditions (22, 23). However, in the time was selected in this study to represent that encountered
presence of chloride, very rapid corrosion (metal polishing) during a typical weekend in many buildings such as schools.
could occur as soluble metal chloride complexes form (23), A mass balance of lead released throughout the study
which occurs for iron if chloride exceeds about 8 M (24). was determined at the end of Case Study 2 for the pure lead
The experimental work that follows attempts to verify the wire apparatus. The scale of the lead wire was carefully
expectations of very low pH and higher anion concentration abraded from the surface using a soft cloth. The lead wire,
in the solder anode microlayer, thereby providing funda- which remained inserted in the 1.3 cm diameter stopper,
mental mechanistic insights to explain practical observations was weighed before and after removal of the scale, and the
of CSMR impacts on lead contamination of potable water collected scale was dissolved with 2% nitric acid and analyzed
from solder. to determine the fraction of lead in the scale. The internal
surface of the upper copper pipe section (1.9 cm diameter)
Experimental Methods was soaked in pH 1.5 water (approximately 0.15% HNO3) for
Pipe Setup. The volume of water in the microlayer contacting 16 h. Following stagnation, the water was removed from each
solder in a real-world pipe joint is extremely small and the pipe, acidiﬁed to a total of 2% nitric acid, and analyzed for
physical contact between the dissimilar metals prevents lead and copper.
measurement of ambient galvanic currents. Therefore, a Analytical Methods. Total lead release was quantiﬁed by
simulated pipe joint corrosion macrocell was designed and acidifying water samples with 2% nitric acid for at least 24 h.
constructed to track changes in water chemistry that result Lead, chloride, and sulfate in the bulk water were measured
from galvanic corrosion between copper pipe and lead solder using an inductively coupled plasma mass spectrometer (ICP-
during stagnation events (Figure 1). This type of apparatus MS) in accordance with Standard Method 3125-B (25).
was shown to semiquantitatively track observed changes in Concentrations of chloride and sulfate were cross-checked
lead leaching due to real-world pipe joints (2). using DIONEX DX-120 ion chromatography according to
The macrocell in this work included a 1.9 cm diameter Standard Method 4110 (25). Chloride microelectrode mea-
copper pipe (31 cm long) and a 1.3 cm diameter copper pipe surements were made with an ion-selective microelectrode
(6.4 cm long), connected by clear Tygon tubing with a 2-mm
by Lazar for Case Studies 1 and 3. Chloride and sulfate
gap separation between the pipes. A 50:50 lead:tin, pure tin,
concentrations used in the calculation of the concentration
or pure lead wire was inserted through the center of a silicone
factors were determined from ICP analysis of “anode” and
stopper, and then the stopper with wire was inserted into
“cathode” water samples. “Anode” samples consisted of the
the 1.3 cm diameter copper pipe. The wetted surface area
of lead solder (or pure lead or pure tin wire) was 6.2 cm2 9-mL solution closest to the solder wire, and “cathode”
(Case Studies 1 and 3) or 5.2 cm2 (Case Study 2). The smaller samples comprised the 10 mL solution withdrawn from
diameter (1.3 cm) copper pipe could be removed to isolate the apparatus top, farthest from the solder wire (Figure 1).
a volume of water near the surface of the anodic solder, The pH of the bulk water was measured before exposure
suitable for measurement of Cl- or SO42-. The larger diameter to the macrocells with an Accumet electrode in accordance
(1.9 cm) pipe had the dual purpose of allowing extraction of with Standard Method 4500-H+ B (25). The pH of the anode
water samples from various depths within the apparatus using (within 1 mm from the solder, Pb, or Sn surface) and cathode
a pipet inserted into the apparatus, and also providing a (in the bulk water in the 1.9 cm diameter copper pipe) was
large copper-to-solder surface area of approximately 34:1 in measured using a ﬂat membrane microelectrode and a
Case Studies 1 and 3 and 41:1 in Case Study 2. To simulate reference electrode from Microelectrodes, Inc. Electrochemi-
the galvanic connection between copper pipes and lead solder cal measurements between the copper pipes and the solder,
in joints while having the ability to measure galvanic corrosion lead, or tin wires were conducted using RadioShack multi-
with an ammeter, each lead or tin bearing wire was externally meters with 100 Ω resistance.
VOL. 44, NO. 18, 2010 / ENVIRONMENTAL SCIENCE & TECHNOLOGY 9 7077
TABLE 1. Bulk Water Chemistry of Test Waters
(case study no.) water type Cl-, mg/L Cl mg/L SO4 CSMRa mg/L as CaCO3 pH inhibitor (dose) disinfectant, mg/L as Cl2
(1) alum-treated 27 21 1.4 25 7.7 orthophosphate various - free chlorine or
(1) PACl-treatedb 32 6 5.3 25 7.7 (1 mg/L P) chloramines (3.5 mg/L)
(1) PACl-treated , simulated road 48 6 8.5 25 7.7
salt runoff (+16 mg/L Cl)
(2) Typical treated water subjected to 4 and 14 3-12 3.0-4.7 8-58 7.3 orthophosphate free chlorine (2 mg/L)
corrosion control strategies (various: 0-1 mg/L P)
(3) low chloride and high sulfate 22 121 0.2 10 8.3 none chloramines (4 mg/L)
(3) high chloride and low sulfate 129 8 16 10 8.3
Chloride-to-sulfate mass ratio (CSMR) is given as mg/L Cl- per mg/L SO42-. b
PACl, polyaluminum chloride.
Results and Discussion
Effect of Galvanic Corrosion on Lead Release. Galvanic
current measured between the anode (solder, lead, or tin
wire) and the cathode (copper pipe) is an indicator of galvanic
corrosion (26). For this study, negative current values
indicated that the lead-tin solder, lead, or tin wires were
anodic (sacriﬁced) while the copper pipes were cathodic
(protected). As the magnitude of the measured galvanic
current increased, lead release to the water increased for
solder wires across all three case studies and for pure lead
wire investigated in the second case study (Figure 2). Lead
release followed a roughly linear relationship with the galvanic
current, consistent with expectations based on Faraday’s law.
This is also consistent with recent work by Sastri et al. who
linked galvanic corrosion to lead leaching from solder in
drinking water (27). In some cases lead concentrations
reached more than 20 000 ppb in the macrocell anode
compartment (results not shown).
For 50:50 Pb/Sn solder, the measured currents reﬂected
not only the corrosion rate of lead but also that of tin. Solder
alloy corrosion may proceed with preferential leaching of
one metal versus the other, but if it is assumed that each
metal corroded at the same rate, the lead released from
50:50 Pb/Sn solder to the water was approximately three
times less than predicted by Faraday’s law for the three case
studies (Figure 2). Similarly, lead release to water from pure
lead wire in Case Study 2 was about 4 times less compared
to the predicted amount, assuming that 100% of the galvanic FIGURE 2. Lead release to bulk water, pH at solder surface,
current was associated with the lead release. However, chloride concentration factor (CF), sulfate CF, and phosphate CF
consistent with Oliphant’s ﬁndings (10), the vast majority of at the anode as a function of galvanic current. The blue dia-
this “missing” lead was found to be accumulated in lead monds, red squares, purple asterisks, and black triangles
scales on the lead anode and elsewhere in the apparatus, as represent Case Study 1 solder, Case Study 2 solder, Case Study
3 solder, and Case Study 2 lead wire, respectively. The solid
conﬁrmed by mass balances at the end of the experiment.
line, dash-dot line, and dashed line represent the linear
Similar trends were observed for tin release from solder and
regression for solder, predicted oxidized lead from solder, and
tin wires. predicted oxidized lead from pure lead wire, respectively.
The potential of the copper pipe was stable ((0.1 V) as Measurements were taken after two days of water stagnation.
the CSMR was varied (results not shown), further conﬁrming The CF is equal to the concentration at the anode divided by
that the electrochemical factors propagating the attack at the concentration at the cathode. The lead measurements were
higher CSMR were occurring at the lead anode surfaces. The taken from the entire volume in the apparatus, while the
actual lead levels released to the water from the apparatus chloride and sulfate concentrations were determined from
used in these case studies was much greater than is observed “anode” and “cathode” volumes (Figure 2). The pH was mea-
in practice, but is in close agreement to prior studies sured within 1 mm of the solder surface using a micro-
examining small volumes of water contacting typical lead electrode. Case Study 2 solder data points include conditions
solder joints in copper pipe (2). with no phosphate, and the lead wire data are the waters with
Anion Migration. Anions such as chloride, sulfate, and 4 and 14 mg/L Cl and alkalinity above 15 mg/L as CaCO3.
phosphate must be drawn to the anode surface to coun-
terbalance released Pb2+ and Sn2+ and maintain electro- calculated by dividing the concentration in the 9 mL of
neutrality (Figure 3). The measured concentrations of these solution closest to the anode by the concentration near the
metals in the water near the anode were as high as 157 000 cathode. As the galvanic corrosion rate increased, the sulfate,
ppb Pb and 41 000 ppb Sn, and cations such as sodium (Na+) phosphate, and chloride CFs increased as electromigration
also migrated toward the cathode, which is the site of OH- became dominant over ion diffusion (Figure 2). For instance,
production (results not shown). Other work by Kim (17) and sulfate was concentrated at the anode surface by a factor of
Horng (16) also measured chloride and sulfate migration to 1.5 when the current density was approximately -1.2 µA/
the anode. Concentration factors (CFs) were used to compare cm2. When the current density quadrupled to -4.8 µA/cm2,
anion accumulation at the anode versus the cathode in this 2.7 times more sulfate was measured in the anode compart-
work and in Horng’s work. The CFs in this study were ment than in the cathodic area of the pipe. Similar trends
7078 9 ENVIRONMENTAL SCIENCE & TECHNOLOGY / VOL. 44, NO. 18, 2010
measurement technique as was observed in the other two
case studies, a chloride concentration factor of 4 was detected
using a microelectrode brought to within 1 mm of the anode
surface. Hence, the actual CFs in the microlayer at the lead
anode surface are likely much larger than reported herein
based on collection of the relatively large water volumes
(≈ 9 mL) near the anode surface. As expected based on the
higher ionic transport numbers of sulfate versus chloride
(28, 29), sulfate had a CF higher than for chloride at a given
current density (Figure 2).
Pure lead and pure tin wires were also evaluated in Case
Study 2. For reasons that are not fully understood, in one
water tested, only sulfate and phosphate accumulated at the
pure lead anode surface, and chloride did not (Figure 2). For
example, the sulfate concentration factor ranged from 0.7 to
3.3 for some water conditions, but there was not a strong
trend between the concentration factor and the galvanic
current density, which ranged from -0.6 to -6.9 µA/cm2.
For pure tin wire in Case Study 2, there was little concentra-
tion of the anions because the current density was nearly
always below 2 µA/cm2.
pH at Anodic Solder Surface. As the galvanic corrosion
rate increased, the pH decreased at the anodic solder surface
due to the Lewis acidity of lead and tin (Figure 2). At the
solder surface after a two-day stagnation period, pH was as
FIGURE 3. pH, chloride concentration, and sulfate concentration low as 3.7 for Case Study 1 and 2.5 for Case Study 3. Some
as a function of distance from the bottom-most part of the measurements indicated that the pH dropped as much as 2
solder anode for Utility 1. The pH and the chloride con- pH units within 1 h of stagnation, demonstrating that days
centrations were measured using a microelectrode. Sulfate of stagnation are not required to observe signiﬁcant galvanic
was measured by withdrawing samples from the apparatus. effects. Even when the galvanic corrosion activity was
The location of the anode was between 0 and 6.4 cm on the relatively low as in Case Study 2, the pH still dropped from
x-axis, and distances greater than 6.4 cm on the x-axis was
pH 7.3 in the bulk water to as low as pH 3.8 at the solder
considered the cathodic region. Error bars represent 95%
surface. The very low pH values measured for solder and tin
conﬁdence intervals over triplicate measurements.
wire were in the range of those predicted by solubility models
(30), considering the Lewis acidity of the detected lead and
tin concentrations. Consistent with expectations and prior
research (31), the pH increased with distance from the anode
due to the net OH- production at the cathode (Figure 3).
Predicted Effect of pH and Anion Migration on Lead
Leaching. To illustrate the effects of chloride and sulfate on
lead solubility at the surface of lead anodes, modeling with
MINEQL+ was conducted. For example, if 50 mg/L Pb(II)
were released to the microlayer of water with 8 mg/L alkalinity
as CaCO3 and the sulfate concentration at equilibrium was
240 mg/L (2.5 mM SO42-), 95% of the released lead is predicted
FIGURE 4. Lead release from 50:50 Pb/Sn solder as a function to form larnakite (PbSO4:PbO) and cerrusite (PbCO3) solid
of the chloride-to-sulfate mass ratio (CSMR) for the case stud- precipitates at pH 6.5 (Figure 5). These solids could coat the
ies. Data from Case Study 2 in the plot represent a range of anode surface and reduce the rate of corrosive galvanic attack.
alkalinity (8-58 mg/L as CaCO3) with and without orthophos- The 240 mg/L SO42- in the microlayer near the lead surface
phate. Water in Case Study 1 was dosed with orthophosphate, could also be obtained by a 10× concentration of 24 mg/L
and treated water in Case Study 3 contained no phosphate. SO42- (0.25 mM) from in the bulk water concentrating 10
times due to electromigration. In contrast, if chloride were
were observed in Horng’s work, although the extent of ion
present at the similar molar concentration mentioned for
migration was less than that measured in this work. Specif-
sulfate in the preceding example, the solubility of lead at the
ically, a current density of -10 µA/cm2 resulted in a sulfate
anode would be increased by 37% to 3.7 mg/L soluble Pb
concentration factor of 1.4 at the anode, and the concentra-
tion factor increased to 5 when the current density increased due to the formation of soluble PbCl+ complexes (Figure 5).
to -25 µA/cm2 (16). The most prominent difference between The relative effect of chloride and sulfate on soluble lead
the two studies is the presence of a cathodic copper surface at the solder surface would be much more dramatic at lower
immediately adjacent to the anode in this work, which would pH values, or with greater concentration factors arising from
tend to decrease the CF versus the microlayer at anode higher galvanic current densities. For example, if 240 mg/L
surfaces in practice, since this portion of the copper surface SO42- and 50 mg/L Pb(II) were added to water at pH 4, only
in the apparatus carried about 50% of the cathodic current. 3.7 mg/L Pb is predicted to remain soluble, while 93% of the
In situations with very low galvanic currents, lead lead would precipitate as PbSO4 which could coat the anode
concentrations were not as strongly impacted by the levels and reduce the corrosion rate (Figure 5). Conversely, chloride,
of chloride and sulfate in the water in this study (ex., Case if present in the microlayer near the anode surface at the
Study 2; Figure 4), consistent with expectations outlined same molar concentration as sulfate in this example, would
earlier. Although CFs greater than one for sulfate and chloride yield 100% soluble lead at the same pH (77% free Pb2+, 15%
in Case Study 3 were not detected with the macrocell PbHCO3+, 8% PbCl+). This explains the beneﬁts of sulfate
VOL. 44, NO. 18, 2010 / ENVIRONMENTAL SCIENCE & TECHNOLOGY 9 7079
C.K.N. was partially supported by a National Science
Foundation (NSF) Graduate Fellowship and a Via Fellowship.
The experimental work was supported by funding from the
Water Research Foundation (WaterRF) and the U.S. EPA,
whereas the advanced analysis of the data and writing of the
manuscript was supported by the NSF under grant CBET-
0933246. The opinions, ﬁndings, conclusions, or recom-
mendations are those of the authors and do not necessarily
reﬂect the views of the WaterRF, NSF, or the U.S. EPA. The
authors also thank Traci Case, Christopher Hill, France
Lemieux, Joseph Marcinko, and Anne Spiesman.
Supporting Information Available
Additional descriptions, ﬁgures, and tables regarding the
bench scale water treatment, tin release, predicted pH,
FIGURE 5. Equilibrium soluble lead concentrations at pH 6.5 chloride concentrations in Case Study 3, potential measure-
(top) and pH 4.0 (bottom) at a lead surface if 50 mg/L Pb(II) is ments, and mass balance of oxidized lead. This material is
released to water with 8 mg/L alkalinity as CaCO3. Sulfate and available free of charge via the Internet at http://pubs.acs.org.
chloride concentrations at the lead surface can be greater than
in bulk water due to electromigration. In water with sulfate,
larnakite (PbSO4:PbO), anglesite (PbSO4), and cerrusite (PbCO3) Literature Cited
solids are predicted to form at pH 6.5, and PbSO4 solids are
(1) Edwards, M.; Dudi, A. Role of chlorine and chloramine in
predicted to begin forming at 0.1 mM SO4 at pH 4.0. If chloride corrosion of lead-bearing plumbing materials. J. Am. Water
were dominant in the water and at the lead anode, PbCO3 and Works Assoc. 2004, 96 (10), 69–81.
Pb(OH)2 solids would form at pH 6.5, and no precipitates are (2) Edwards, M.; Triantafyllidou, S. Chloride-to-sulfate mass ratio
predicted to form at pH 4.0. and lead leaching to water. J. Am. Water Works Assoc. 2007, 99
(3) Giammar, D. In Inﬂuence of Water Chemistry on the Dissolution
and the detrimental effect of chloride in preventing lead Rates of Lead Corrosion Products Proceedings of American Water
contamination of potable water in lead solder:copper joints Works Association Water Quality Technology Conference, Seattle,
(Figure 4). WA, November 15 2009; American Water Works Association:
In the present study, all of the lead would be leached Denver, CO, 2009.
(4) Lytle, D. A.; Schock, M. R. Formation of Pb(IV) oxides in
from the solder wires in Case Study 2 after the experiment
chlorinated water. J. Am. Water Works Assoc. 2005, 97 (11), 102–
continued 5-630 years, based on the galvanic currents from 114.
Week 15 of the study. In practice, the quality of soldering (5) Schock, M. R.; Swertfeger, J.; Harmon, S. M.; Lohmann, R.;
workmanship varies from home to home, as exposed solder DeMarco, J. In Tetravalent lead: A hitherto unrecognized control
at a given pipe joint can range from a nearly negligible mass of tap water lead contamination, Proceedings of American Wa-
ter Works Association Water Quality Technology Conference,
to well over 10 g (32). Thus, the self-perpetuating corrosion Nashville, TN, November 11-14, 2001; American Water Works
can be very serious in some situations and can require Association: Denver, CO, 2001.
adjustment of the CSMR back to lower ranges to reduce lead (6) Edwards, M.; Triantafyllidou, S.; Best, D. Elevated blood lead
leaching to below the USEPA LCR action level of 15 ppb (2). in young children due to lead-contaminated drinking water:
Implications for Drinking Water Systems. Galvanic Washington, DC, 2001-2004. Environ. Sci. Technol. 2009, 43
reactions can drive corrosion of lead metal at copper joints (7) Miranda, M. L.; Kim, D.; Hull, A. P.; Paul, C. J.; Galeano, M. A.
and contribute to exceedance of the U.S. EPA LCR (2, 15). Changes in blood lead levels associated with use of chloramines
Furthermore, in waters supporting relatively high galvanic in water treatment systems. Environ. Health Perspect. 2007,
currents, higher chloride and lower sulfate can worsen 115 (2), 221–225.
(8) Renner, R. Mapping out lead’s legacy. Environ. Sci. Technol.
corrosion of lead solder, which is believed to be the dominant 2009, 43 (6), 1655–1658.
source of lead in water in many situations (11). The detriments (9) Gregory, R. Galvanic corrosion of lead solder in copper pipework.
of chloride are attributed to its migration to the anode surface Water Environ. J. 1990, 4 (2), 112–118.
and formation of soluble PbCl+ complexes, whereas the (10) Oliphant, R. J. Summary Report on the Contamination of Potable
beneﬁts of sulfate may be attributed to formation of relatively Water by Lead from Soldered Joints; 125E; Water Research Centre:
Wiltshire, UK, November,1983.
insoluble PbSO4 (or similar) solids. This work is the ﬁrst to (11) American Water Works Association Research Foundation.
demonstrate the very large gradation in pH, chloride, sulfate, Internal Corrosion of Water Distribution Systems, 2nd ed.;
and lead that can be produced via galvanic corrosion of lead American Water Works Association: Denver, CO, 1996.
solder:copper joints under stagnant water conditions, which (12) Reiber, S. Galvanic stimulation of corrosion on lead-tin solder
sweated joints. J. Am. Water Works Assoc. 1991, 83 (7), 83–91.
can often exceed 48 h duration over weekends in building
(13) Edwards, M.; Jacobs, S.; Dodrill, D. Desktop guidance for
plumbing systems. Recently, similar conclusions about low mitigating Pb and Cu corrosion by-products. J. Am. Water Works
local pH, high chloride, high sulfate, and very high lead in Assoc. 1999, 91 (5), 66–77.
microenvironments near surfaces of lead anodes were drawn (14) Dudi, A. Reconsidering Lead Corrosion in Drinking Water:
by Desantis et al., based on independent mineralogical Product Testing, Direct Chloramines Attack and Galvanic
Corrosion. Master’s Thesis, Virginia Tech, Blacksburg, VA, 2004.
examination of lead:copper pipe connections from extracted
(15) Nguyen, C. K.; Stone, K. R.; Edwards, M. A. Chloride-to-sulfate
service line samples (20). In sum, these microlayer effects mass ratio: Practical studies in lead solder galvanic corrosion.
can explain a subset of persistent lead corrosion problems J. Am. Water Works Assoc. 2010. In Press.
in some buildings and from lead:copper service line joints (16) Horng, J.-J. A Model Study of Ionic Transport and Its Role in
at some water utilities (2). Additional work is needed to better Electrokinetic Treatment of Contaminated Soils. Doctoral
Dissertation, University of Washington, Seattle, 1993.
understand situations in which persistent galvanic currents (17) Kim, K.-J.; Cho, J.-M.; Baek, K.; Yang, J.-S.; Ko, S.-H. Electrokinetic
occur, and how they can be practically mitigated through removal of chloride and sodium from tidelands. J. Appl.
control of water chemistry. Electrochem. 2010.
7080 9 ENVIRONMENTAL SCIENCE & TECHNOLOGY / VOL. 44, NO. 18, 2010
(18) Lim, K.-H.; Franses, E. I., Change in overall ohmic resistance (25) American Public Health Association (APHA). Standard Methods
due to migration/diffusion of electrolytes. In Electrochemical for the Examination of Water and Wastewater, 20th ed.; APHA,
Cell Design, White, R. E., Ed.; Plenum Press: Houston, TX, American Water Works Association, and Water Environment
1984. Federation: Washington, D.C., 1998.
(19) Schock, M. R. Understanding corrosion control strategies for (26) ASTM Standard G71-81, Standard Guide for Conducting and
lead. J. Am. Water Works Assoc. 1989, 81 (7), 88–100. Evaluating Galvanic Corrosion Tests in Electrolytes; ASTM
(20) DeSantis, M. K.; Welch, M. M.; Schock, M. R. In Mineralogical International: West Conshohocken, PA, 2009.
evidence of galvanic corrosion in domestic, drinking water (27) Sastri, V. S.; Subramanian, K. S.; Elboujdaini, M.; Perumareddi, J. R.
pipes, Proceedings of American Water Works Association Water Inhibition of release of lead into water owing to galvanic corrosion
Quality Technology Conference, Seattle, WA, November 15- of lead solders. Corros. Eng. Sci. Technol. 2006, 41 (3), 249–254.
19, 2009; American Water Works Association: Denver, CO, (28) Tower, O. F. The Conductivity of Liquids: Methods, Results,
2009. Chemical Applications, and Theoretical Considerations; Chemi-
cal Publishing Company: Easton, PA, 1905.
(21) Nguyen, C.; Edwards, M.; Stone, K.; Clark, B. In Mechanistic
(29) Arrhenius, S. Textbook of Electrochemistry; Longmans, Green,
effects of chloride-to-sulfate ratio on lead corrosion, Proceedings
and Co.: New York, NY, 1902.
of American Water Works Association Annual Conference and
(30) Schecher, W. D.; McAvoy, D. C. MINEQL+: A Chemical Equi-
Exposition, Atlanta, GA, June 8-12, 2008; American Water Works
librium Modeling System. Version 4.0 for Windows; Environ-
Association: Denver, CO, 2008.
mental Research Software: Hallowell, ME.
(22) Guo, Y. A new potential-pH diagram for an anodic ﬁlm on Pb (31) Kuhn, A. T.; Chan, C. Y. pH changes at near-electrode surfaces.
in H2SO4. J. Electrochem. Soc. 1992, 139 (8), 2114–2120. J. Appl. Electrochem. 1983, 13 (2), 189–207.
(23) Sato, N. Interfacial ion-selective diffusion layer and passivation (32) Economic and Engineering Services. Lead Control Strategies;
of metal anodes. Electrochim. Acta 1996, 41 (9), 1525–1532. Water Research Foundation: Denver, CO, 1990.
(24) Sato, N. The stability of localized corrosion. Corros. Sci. 1995,
37 (12), 1947–1967. ES1015185
VOL. 44, NO. 18, 2010 / ENVIRONMENTAL SCIENCE & TECHNOLOGY 9 7081